322 PHENOLIC RESINS Vol. 7PHENOLIC RESINSIntroductionPhenolic resins are a large family of polymers and oligomers, composed of a widevariety of structures based on the reaction products of phenols with formaldehyde.Phenolic resins are employed in a wide range of applications, from commodity con-struction materials to high technology applications in electronics and aerospace.Generally, but not exclusively, thermosetting in nature, phenolic resins provide nu-merous challenges in the areas of synthesis, characterization, production, productdevelopment, and quality control. As a family of resins originally developed in the early twentieth century, thenature and potential of phenolic resins have been explored thoroughly to producean extensive body of technical literature (1–9). A symposium sponsored by theAmerican Chemical Society commemorated 75 years of phenolic resin chemistry in1983 (10), and in 1987 the Phenolic Molding Division of the Society of the PlasticsIndustry (SPI) sponsored a conference on phenolics in the twenty-ﬁrst century (1).Exciting new developments continue as new systems are developed for carbon–carbon composites, aramid honeycombs, and new derivative chemistries such ascyanate esters and benzoxazines. New U.S. patents with phenolic resins in theclaims are growing at about 150 patents per year. Phenolic resins are prepared by the reaction of phenol or substituted phenolwith an aldehyde, especially formaldehyde, in the presence of an acidic or basiccatalyst. Their thermosetting character and the exotherm associated with thereaction presented technical barriers to commercialization. In 1900, the ﬁrst U.S.patent was granted for a phenolic resin, using the resin in cast form as a substitutefor hard rubber (11). Work on the ﬁrst commercially viable product was initiated by Baekelandin 1905. Using phenol and formaldehyde as starting materials, he establishednot only the differences between acid- and alkali-catalyzed products, but also theimportance of excess phenol or formaldehyde made in producing intermediates.Encyclopedia of Polymer Science and Technology. Copyright John Wiley & Sons, Inc. All rights reserved.
Vol. 7 PHENOLIC RESINS 323However, producing the resin was only part of the challenge. Baekeland also de-veloped the technology to convert the reactive resins, which had a severe tendencyto foam and cure to a brittle product, into useful molded articles by adding woodor mineral ﬁbers and molding under heat and pressure. The ﬁnal molded partswere tough, temperature resistant, and had a low void content (12). The ﬁrst com-mercial phenolic resin plant was Bakelite GmbH, started in Germany in 1910; inthe same year, the General Bakelite Co. was founded in the United States. Early phenolic resins consisted of self-curing, resole-type products made withexcess formaldehyde, and novolaks, which are thermoplastic in nature and requirea hardener. The early products produced by General Bakelite were used in moldedparts, insulating varnishes, laminated sheets, and industrial coatings. These ar-eas still remain important applications, but have been joined by numerous otherssuch as wood bonding, ﬁber bonding, and plywood adhesives. The number of pro-ducers in 2001 is approximately 15 in the United States and over 50 worldwide.Overall the number of producers is declining as the industry continues to undergoconsolidation.Monomers Phenol. This is the monomer or raw material used in the largest quantityto make phenolic resins (Table 1). As a solid having a low melting point, phenol,C6 H5 OH, is usually stored, handled in liquid form at 50–60◦ C, and stored undernitrogen blanket to prevent the formation of pink quinones. Iron contaminationresults in a black color. The most widely used process for the production of phenol is the cumeneprocess developed and licensed in the United States by Honeywell (formerlyAlliedSignal). Benzene is alkylated with propylene to produce cumene (isopropyl-benzene), which is oxidized by air over a catalyst to produce cumene hydroperoxide(CHP). With acid catalysis, CHP undergoes controlled decomposition to producephenol and acetone; α-methylstyrene and acetophenone are the by-products (13).Other commercial processes for making phenol include the Raschig process, usingchlorobenzene as the starting material, and the toluene process, via a benzoic acidintermediate. In the United States, ∼35–40% of the phenol produced is used forphenolic resins. Table 1. Properties of Phenol Property Value mol wt 94.1 mp, ◦ C 40.9 bp, ◦ C 181.8 Flash point, ◦ C 79.0 Autoignition temperature, ◦ C 605.0 Explosive limits, vol% 2–10 Vapor pressure at 20◦ C, Paa 20 a To convert Pa to mm Hg, multiply by 7.5 × 10 − 3 .
324 PHENOLIC RESINS Vol. 7 Table 2. Substituted Phenols Used for Phenolic Resins Substituted phenol Resin application Cresol (o-, m-, p-) Coatings, epoxy hardeners p-t-Butylphenol Coatings, adhesives p-Octylphenol Carbonless paper, coatings p-Nonylphenol Carbonless paper, coatings p-Phenylphenol Carbonless paper Bisphenol A Low color molding compounds, coatings Resorcinol Adhesives Cashew nutshell liquid Friction particles Substituted Phenols. Phenol itself is used in the largest volume, butsubstituted phenols are used for specialty resins (Table 2). Substituted phenolsare typically alkylated phenols made from phenol and a corresponding α-oleﬁnwith acid catalysts (14). Acidic catalysis is frequently in the form of an ion-exchange resin (IER) and the reaction proceeds preferentially in the para position.For example, in the production of t-butylphenol using isobutylene, the product is>95% para-substituted. The incorporation of alkyl phenols such as cresol into theresin reduces reactivity, hardness, cross-link density, and color formation, but in-creases solubility in nonpolar solvents, ﬂexibility, and compatibility with naturaloils. Formaldehyde. In one form or another, formaldehyde is used almost ex-clusively in the production of phenolic resins, regardless of the type of phenol(Table 3). It is frequently produced near the site of the resin plant by either of twocommon processes using methanol (qv) as the raw material. In the silver catalystprocess, the reaction takes place at 600–650◦ C and produces water and hydrogenas by-products. The more common metal oxide process operates at 300–400◦ C.The gaseous formaldehyde is absorbed in water, and the ﬁnal product is a for-malin solution containing 36–50% formaldehyde. Of the various chemical formsof formaldehyde, the aqueous form is preferred for making phenolic resins, eventhough at least half of this form is water. The water serves to moderate the reactionand is readily removed in processing equipment (15). Aqueous Formaldehyde. Water solutions of formaldehyde consist mainlyof telomers of methylene glycol having <100 ppm of the formaldehyde as CH2 O (5).Alcohols form hemiformals with aqueous formaldehyde according to the following,where n = 1, 2, 3, etc. ROH + HOCH2 OH ROCH2 OH + H2 O RO(CH2 O)nH + HOCH2 OH RO(CH2 O)n + 1 H + H2 OHowever, a second mole of alcohol or hemiformal does not add at the ordinarypH of such solutions. The equilibrium constant for hemiformal formation de-pends on the nature of the R group of the alcohol. Using NMR spectroscopy, agroup of alcohols including phenol has been examined in solution with formalde-hyde (16,17). The spectra indicated the degree of hemiformal formation in the
Vol. 7 PHENOLIC RESINS 325Table 3. Forms of Formaldehyde Resin preparationType Chemical formula Advantages DisadvantagesGaseous CH2 O UnstableFormalin36% HO(CH2 O)n Ha Easy handling, High water moderate, content reactivity, stable at RT50% HO(CH2 O)n Hb Increased capacity Elevated temperature storage, formic acid formationParaformaldehyde HO(CH2 O)n Hc Increased Dangerously high capacity, reactivity, solids water-free handlingTrioxane (CH2 O)3 Water-free Catalyst requirements, high costHexamethylenetetramine (CH2 )6 N4 Autocatalytic Amine incorporationan ≈ 2.bn ≈ 3.c n = 20–100.order of methanol > benzyl alcohol > phenol. Hemiformal formation provides themechanism of stabilization; methanol is much more effective than phenol in thisregard. The large value for the hemiformal formation constant of methanol and itslow molecular weight explains the high efﬁciency of methanol in stabilizing for-malin solutions. Phenol, on the other hand, is inefﬁcient, and phenol hemiformalsare only formed by careful removal of water (18). Other Aldehydes. The higher aldehydes react with phenol in much thesame manner as formaldehyde, although at much lower rates. Examples includeacetaldehyde, CH3 CHO; paraldehyde, (CH3 CHO)3 ; glyoxal, OCH CHO; and fur-fural. The reaction is usually kept on the acid side to minimize aldol formation.Furfural resins, however, are prepared with alkaline catalysts because furfuralself-condenses under acid conditions to form a gel. Hexamethylenetetramine. Hexa, a complex molecule with anadamantane-type structure, is prepared from formaldehyde and ammonia,and can be considered a latent source of formaldehyde. When used either as acatalyst or as a curative, hexa contributes formaldehyde-residue-type units aswell as benzylamines. Hexa [100-97-0] is an infusible powder that decomposesand sublimes above 275◦ C. It is highly soluble in water, up to ca 45 wt% witha small negative temperature solubility coefﬁcient. The aqueous solutions aremildly alkaline at pH 8–8.5 and reasonably stable to reverse hydrolysis.
326 PHENOLIC RESINS Vol. 7 Other Reactants. Other reactants are used in smaller amounts to providephenolic resins that have speciﬁc properties, especially coatings applications. Ani-line had been incorporated into both resoles and novolaks but this practice hasbeen generally discontinued because of the toxicity of aromatic amines. Othermaterials include rosin (abietic acid), dicyclopentadiene, unsaturated oils such astung oil and linseed oil, and polyvalent cations for cross-linking.PolymerizationPhenolic resins are prepared with strong acid or alkaline catalysts. Occasionally,weak or Lewis acids, such as zinc acetate, are used for specialty resins. Strong-Acid Catalysts, Novolak Resins. Phenolic novolaks are ther-moplastic resins having a molecular weight of 500–5000 and a glass-transitiontemperature T g of 45–70◦ C. The phenol–formaldehyde reactions are carried totheir energetic completion, allowing isolation of the resin; formaldehyde–phenolmolar ratios are between 0.5:1 and 0.8:1. Methylene glycol [463-57-0] (1) is con-verted to the corresponding hydrated carbonium ion 2, which adds to the ortho andpara positions of phenol with the elimination of water to form the correspondingortho (3) and para (4) benzylic ions. The benzylic carbonium ions are in equi-librium with the corresponding benzylic alcohols, observed by NMR as transientspecies in the formation of novolak resins (16). In the next step the hydrated benzylic carbonium ions 3 and 4 react with freeortho and para positions on phenols to form methylene-linked bisphenols, 2,2 (5),2,4 (6), and 4,4 (7).
Vol. 7 PHENOLIC RESINS 327 Table 4. Novolak Resin Properties Catalyst Property Acid Zn acetatea Formaldehyde/phenol molar ratio 0.75 0.60 NMR analysis, % 2,2 6 45 2,4 73 45 4,4 21 10 GPC analysis Phenol, % 4 7 Mn 900 550 Mw 7300 1800 Water, % 1.1 1.9 Tg , ◦ C 65 48 Gel time, s 75 25 a High ortho. Continued reaction leads to the formation of novolak polymers having amolecular weight of up to 5000. Acid-catalyzed resins contain 50–75% 2,4 link-ages (6). The reaction rate is proportional to catalyst, formaldehyde, and phenolconcentrations, and inversely proportional to the concentration of water. The rateof formation of the benzyl alcohol intermediate is 5–10 times lower than the rateto form the methylene-linked bisphenol (3). At typical molecular weights of 500–1000, novolak molecules are essentially linear because of the much lower reactiv-ity of doubly-reacted phenolic units. In higher molecular weight polymers, the lowconcentration of end groups and unreacted phenol causes branching. Above 1000molecular weight, branching has been observed by 13 C NMR; about 20% branch-ing has been predicted in computer simulations (14,19,20). In the curing process,end groups are more reactive than the backbone groups. Thus a branched resinhaving a higher content of end groups than a corresponding linear equivalent maygel sooner and cure faster because of the higher resin functionality. The propertiesof an acid-catalyzed phenolic resin are shown in Table 4. The typical acid catalysts used for novolak resins are sulfuric acid, sulfonicacid, oxalic acid, or occasionally phosphoric acid. Hydrochloric acid, althoughonce widely used, has been abandoned because of the possible formation of toxicchloromethyl ether by-products. The type of acid catalyst used and reaction condi-tions affect resin structure and properties. For example, oxalic acid, used for resinschosen for electrical applications, decomposes into volatile by-products at elevatedprocessing temperatures. Oxalic acid catalyzed novolaks contain small amounts(1–2% of the original formaldehyde) of benzodioxanes formed by the cyclizationand dehydration of the benzyl alcohol hemiformal intermediates.
328 PHENOLIC RESINS Vol. 7 Benzodioxane is reasonably stable at neutral pH, but may decompose whenthe resin is cured, serving as a source of labile formaldehyde. Benzodioxanes arenot found in sulfuric or sulfonic acid catalyzed resins, since the stronger acidreadily catalyzes the second step in the reaction sequence. Neutral Catalysts, High Ortho Novolaks. In the range of pH 4–7,formaldehyde substitution of the phenolic ring is possible, using divalent metalcatalysts containing Zn, Mg, Mn, Cd, Co, Pb, Cu, and Ni; certain aluminum saltsare also effective. Organic carboxylates are required as anions in order to obtainsufﬁcient solubility of the catalyst in the reaction medium, as well as to provide aweak base. Acetates are most convenient and economical. Although lead acetateis highly effective because of its excellent solubility properties, it has been largelyeliminated because of lead toxicity. Zinc and calcium salts are probably the mostwidely used catalysts (21). Novolaks produced from these catalysts exhibit a high content of 2,2 -methylene units. The mechanism proposed for the ortho-directing effect involveschelation of the phenolic unit with the metal ion.Zinc acetate catalyst produces essentially 100% o-methylol phenol (8) in the ﬁrststep. The second step gives an approximately equal quantity of 2,2 - (5, 45%) and2,4%-diphenylmethylene (6, 45%) bridges, indicating little chelate-directing inﬂu-ence. In addition, a small quantity (10%) of methylene ether units (9) (dibenzylether) is observed at moderate reaction temperature. High ortho novolaks have faster cure rates with hexa. Typical properties of azinc acetate catalyzed high ortho novolak are also shown in Table 4. The gel timewith hexa is one-third of that with a strong acid catalyzed novolak. Alkaline Catalysts, Resoles. Resole-type phenolic resins are producedwith a molar ratio of formaldehyde to phenol of 1.2:1 to 3.0:1. For substitutedphenols, the ratio is usually 1.2:1 to 1.8:1. Common alkaline catalysts are NaOH,Ca(OH)2 , and Ba(OH)2 . While novolak resins and strong acid catalysis result in alimited number of structures and properties, resoles cover a much wider spectrum.Resoles may be solids or liquids, water-soluble or -insoluble, alkaline or neutral,slowly curing or highly reactive. In the ﬁrst step, the phenolate anion is formedby delocalization of the negative charge to the ortho and para positions. Alkalinecatalysts are also effective in the polymerization–depolymerization of methylene
Vol. 7 PHENOLIC RESINS 329glycol. The mechanism of the formaldehyde addition to the phenolate is still notcompletely understood. The most likely mechanism involves the contribution ofphenol hemiformals (10) (5). Rate studies show that base-catalyzed reactions are second order and de-pend on the phenolate and methylene glycol concentrations. The most likely pathinvolves a nucleophilic displacement by the phenoxide on 1, with the hydroxyl asthe leaving group. In alkaline media, the methylolated quinone intermediate isreadily converted to the phenoxide by hydrogen-ion abstraction (22). The ratio of ortho-to-para substitution depends on the nature of the cationand the pH. Para substitution is favored by K+ and Na+ ions and higher pH,whereas ortho substitution is favored at lower pH and by divalent cations, suchas Ba2+ , Ca2+ , and Mg2+ (23). Several extensive kinetic studies on the polymethylolation of phenol havebeen reported (22,24,25). For the reaction scheme shown in Fig. 1, seven differ-ent rate constants must be determined. Despite different solution concentration,temperatures, and methods of analysis, comparing reaction rates (26–28) fromeach study using an NaOH catalyst gave fairly close agreement that rate con-stants increase with methylol substitution. In fact, dimethylol-substituted phe-nols react with formaldehyde two to four times faster than phenol. As a re-sult, unreacted phenol remains high in resole resins (5–15%) even though theformaldehyde/phenol ratio is as high as 3:1. Fig. 1. Possible pathways and rate constants for the methylolation of phenol.
330 PHENOLIC RESINS Vol. 7 The rate studies show that k264 is by far the fastest reaction (by a factor of4–6) than k2 or k4 , with k24 the second fastest (by a factor of 2–4) (22,25). Although monomeric methylolated phenols are used in certain applications,such as in ﬁber bonding, higher molecular weight resins are usually desirable.Molecular weight is increased by further condensation of the methylol groups,sometimes after the initial pH has been reduced. Dibenzyl ether (9) and diphenyl-methylene formation are shown in the following. The formation of diphenylmethy-lene bridges is favored above 150◦ C and under strongly alkaline conditions; diben-zyl ether formation is favored at lower temperatures and near neutral pH. Special resoles are obtained with amine catalysts, which affect chemical andphysical properties because amine is incorporated into the resin. For example, thereaction of phenol, formaldehyde, and dimethylamine is essentially quantitative(29).In practice, ammonia is most frequently used. With hexa, the initial reactionsteps differ, but the ﬁnal resole resins are identical, provided they contain thesame number of nitrogen and CH2 groups. Most nitrogen from ammonia or hexa isincorporated as dibenzylamine with primary, tertiary, and cyclic amine structuresas minor products. The physical properties of a resole resin prepared with hexa catalyst areshown in Table 5. Compared to the resin catalyzed with NaOH, this resin hashigher molecular weight, less free phenol, lower water solubility, and a higher T g .
Vol. 7 PHENOLIC RESINS 331 Table 5. Properties of Resole Resins Catalyst Property NaOH Hexa Concentration, pph 3 10 Formaldehyde/phenol ratio 2.0 1.5 Water solubility, % 100 Swells GPC analysis Phenol, % 6 8 Mn 280 900 Mw 500 3000 Tg , ◦ C 35 47 Gel time, s 65 110 Table 6. Methylene Group Distribution, % in Resoles Catalyst Methylene group NaOH Hexaa 2-CH2 OH 30 24 2-CH2 OCH2 OH 24 1 2-CH2 OR 2 4 4-CH2 OH 12 9 4-CH2 OCH2 OH 16 0 4-CH2 OR 2 4 2,2 -CH2 0 0 2,4 -CH2 7 12 4,4 -CH2 7 10 2-CH2 N 0 27 4-CH2 N 0 7 Benzoxazine 0 2 a6 pph.This increase in T g is higher than that expected if only phenol and formaldehydewere used, and is a result of the hydrogen-bonding interaction between the back-bone amine units and the phenolic hydroxyls. Taking advantage of this effect,hexa and ammonia have been frequently used to produce solid, grindable, andwater-insoluble resoles for molding compounds. The methylene-isomer distributions of NaOH and hexa-catalyzed resoles areshown in Table 6. The distribution of amine structures is secondary > primary ≈ tertiaryand most benzylamines are ortho in the phenol ring from early steps in the reactionsequence.
332 PHENOLIC RESINS Vol. 7 Weigh tanks Formaldehyde Phenol Safety blow-off Water-cooled condenser Vacuum Safety rupture disk Distillate Motor receiver Vapor Temperature column recorder Sample port and Jacket steam catalyst addition or cooling water Resin coolers for solid one-steps; resin pans or flaker for novolaks Fig. 2. Typical phenolic resin production unit.ManufactureThe ﬁnal state of a phenolic resin varies dramatically from thermoplastic to ther-moset and from solid to liquid, and includes solutions and dispersions. With abulk process, resole resins, in neat or concentrated form, must be produced insmall batches (≈ 2–10 m3 ) in order to maintain control of the reaction and obtaina uniform product. On the other hand, if the product contains a large amount ofwater, such as liquid plywood adhesives, large reactors (20 m3 ) can be used. Melt-stable products such as novolaks can be prepared in large batches (20–40 m3 ) ifthe exotherms can be controlled. Some reactors are reportedly as large as 60 m3(Ref. 9, p. 83). Batch processes for most phenolic resins employ the equipment shown inFig. 2. Liquid reactants are metered into the stirred reaction vessel through weightanks, whereas solid reactants such as bisphenol A and Ba(OH)2 present handlingproblems. Facilities are provided to carry out the reaction under vacuum or aninert gas. Materials of Construction. Compatibility of the materials of construc-tion and the process chemicals is extremely important. The reactors are usuallymade of stainless steel alloys. Copper is avoided because of the possible presence
Vol. 7 PHENOLIC RESINS 333of amines. Glass-lined reactors are occasionally used for nonalkaline resins. Be-cause the use of HCl has been largely discontinued, material requirements are lessstringent. The reactor contains a bottom discharge, which for solid heat-reactiveresins must be large. Solid resole resins are discharged for rapid cooling in or-der to quench the thermosetting reactions. Resin coolers are made up of verticalplates with internally circulating water. The product can also be discharged to alarge cooled surface. Discharges to belt and drum ﬂakers are highly automated;however they can only be used for less-reactive resins. Novolak resins can be stored molten in heated holding tanks under nitrogen.Because novolaks are used mainly in pulverized form with hexa and additives, aprocess that includes belt ﬂaking and feeding directly into the blending and pul-verizing system is preferred. Liquid and solution resole resins are cooled in thereactor by using jacket cooling and vacuum reﬂuxing. Discharged products areﬁltered and pumped to refrigerated intermediate holding areas or packaged forshipping. The stability of liquid resole products varies greatly from product toproduct and depends on the storage temperature. The viscosity of a liquid resoleresin increases but the water miscibility decreases as time and temperature in-crease. Generally, resoles, both liquids and solids, must be refrigerated. Novolak Resins. In a conventional novolak process, molten phenol isplaced into the reactor, followed by a precise amount of acid catalyst. The formalde-hyde solution is added at a temperature near 90◦ C and a formaldehyde-to-phenolmolar ratio of 0.75:1 to 0.85:1. For safety reasons, slow continuous or stepwise ad-dition of formaldehyde is preferred over adding the entire charge at once. Reactionenthalpy has been reported to be above 80 kJ/mol (19 kcal/mol) (30,31). The heatof reaction is removed by reﬂuxing the water combined with the formaldehyde orby using a small amount of a volatile solvent such as toluene. Toluene and xyleneare used for azeotropic distillation. Following decantation, the toluene or xyleneis returned to the reactor. The reaction is completed after 6–8 h at 95◦ C; volatiles, water, and somefree phenol are removed by vacuum stripping up to 140–170◦ C. For resins requir-ing phenol in only trace amounts, such as epoxy hardeners, steam distillation orsteam stripping may be used. Both water and free phenol affect the cure and ﬁnalresin properties, which are monitored in routine quality control testing by gaschromatography (GC). Oxalic acid (1–2 parts per 100 parts phenol) does not re-quire neutralization because it decomposes to CO, CO2 , and water; furthermore,it produces milder reactions and low color. Sulfuric and sulfonic acids are strongcatalysts and require neutralization with lime; 0.1 parts of sulfuric acid per 100parts of phenol are used. A continuous process for novolak resin production hasbeen described (32,33). An alternative process for making novolaks without acidcatalysis has also been reported (34,35), which uses a peroxidase enzyme to poly-merize phenols in an aqueous solution. The enzyme can be derived from soybeansor horseradish. High Ortho Novolaks. The process for high ortho novolaks is similar tothe one used for those catalyzed by strong acid. Zinc acetate is used at concen-trations higher than the acids, typically 2% or more. The formaldehyde/phenolratio is similar (0.75–0.85) but yields are 5–10% lower than those produced withstrong acids, and reaction times are longer. Problems with gel particles and bulkgelation occur more frequently because small amounts of reactive dibenzyl ether
334 PHENOLIC RESINS Vol. 7groups are present. Overall, the process is more expensive because of higher rawmaterial costs, lower yields, and longer cycle times. Another process employs a pH maintained at 4–7 and a catalyst that com-bines a divalent metal cation and an acid. Water is removed continuously byazeotropic distillation and xylene is recycled. The low water content increasesthe reaction rate. The dibenzyl ether groups are decomposed by the acid; the yieldof 2,2 -methylene can be as high as 97% (36). Resoles. Like the novolak processes, a typical resole process consists ofreaction, dehydration, and ﬁnishing. Phenol and formaldehyde solution are addedall at once to the reactor at a molar ratio of formaldehyde to phenol of 1.2–3.0:1.Catalyst is added and the pH is checked and adjusted if necessary. The catalystconcentration can range from 1 to 5% for NaOH, 3 to 6% for Ba(OH)2 , and 6 to 12%for hexa. A reaction temperature of 80–95◦ C is used with vacuum-reﬂux control.The high concentration of water and lower enthalpy compared to novolaks allowsbetter exotherm control. In the reaction phase, the temperature is held at 80–90◦ C and vacuum-reﬂuxing lasts from 1 to 3 h as determined in the developmentphase. Solid resins and certain liquid resins are dehydrated as quickly as possibleto prevent overreacting or gelation. The endpoint is found by monitoring the geltime, which decreases as the reaction progresses. Automation includes on-lineviscosity measurement, GC, and gel-permeation chromatography (GPC). Phenolic Dispersions. These systems are predominantly resin-in-watersystems in which the resin exists as discrete particles. Particle size ranges from0.1 to 2 µm for stable dispersions and up to 100 µm for dispersions requiringconstant agitation. Some of the earliest nonaqueous dispersions were developedfor coatings applications. These systems consist of an oil-modiﬁed phenolic resincomplexed with a metal oxide and a weak solvent. In the postdispersion process, the solid phenolic resin is added to a mixtureof water, cosolvent, and dispersant at high shear mixing, possibly with heating.The cosolvent, frequently an alcohol or glycol ether, and heat soften the resinand permit small particles to form. On cooling, the resin particles, stabilized bydispersant and perhaps thickener, harden and resist settling and agglomeration.Both resole and novolak resins have been made by this process (26). The in situ process is simpler because it requires less material handling (37);however, this process has been used only for resole resins. When phenol is used, thereaction system is initially one-phase; alkylated phenols and bisphenol A presentspecial problems. As the reaction with formaldehyde progresses at 80–100◦ C, theresin becomes water-insoluble and phase separation takes place. Catalysts suchas hexa produce an early phase separation, whereas NaOH-based resins retainwater solubility to a higher molecular weight. If the reaction medium contains aprotective colloid at phase separation, a resin-in-water dispersion forms. Alterna-tively, the protective colloid can be added later in the reaction sequence, in whichcase the reaction mass may temporarily be a water-in-resin dispersion. The pro-tective colloid serves to assist particle formation and stabilizes the ﬁnal particlesagainst coalescence. Some examples of protective colloids are poly(vinyl alcohol),gum arabic, and hydroxyethylcellulose. For products intended to remain stable dispersions for an extended period,a particle size of 2 µm or less is desirable. A thickening agent is usually addedafter the reaction has been completed and the mixture is cooled in order to prevent
Vol. 7 PHENOLIC RESINS 335settling and agglomeration. Examples of thickeners are guar gum, xanthan gum,and hydroxyethylcellulose. The ﬁnal products are generally between 40 and 50%solids, with a viscosity of 1500–5000 mPa·s (=cP). Resole dispersions intended for isolation as discrete particles (27) can beused as ﬂatting agents in coatings (28). Particles larger than 1000 µm are usedin friction-element compositions. A-stage, thermosetting phenolic particles havebeen isolated from dispersion (27,38). With a hexa catalyst (6–12 parts) and aformaldehyde/phenol ratio of 1.5:1, the reaction is carried out at 50% solids for≈ 90 min at 85◦ C. Poly(vinyl alcohol) and gum arabic are the preferred protectivecolloids. The particles (20–80 µm) are isolated from the mixture by ﬁltration and,in the patent examples, by ﬂuid-bed drying. These A-stage products (gel time at150◦ C, 50–100 s) are suitable in applications where pulverized phenolic resins arebeing used, as well as in applications that take advantage of their spherical nature.One patent describes a sinter-resistant product for wood-bonding applications(39). In another patented process, both the production of particulate novolak resinsand the aqueous dispersions of these resins are described (40). Spray-Dried Resins. Spray drying produces resins in particulate form.Spray-drying a resole solution containing a blowing agent (41) produces pheno-lic microballoons. Spray drying also produces A-stage resins (42). The resins,prepared with a high NaOH content, are spray dried to give a ﬁnal particlesize of 40–60 µm. The particles are hygroscopic because of the high causticcontent, but are sinter-resistant when kept dry. The principal application forthis type of product is believed to be wood binding, especially for waferboardapplications. Cyanate Ester Resins. Cyanate ester resins, sometimes called triazinesor cyanurates after the cured structure that they produce, are derived fromphenols and phenolic resins. Speciﬁcally the starting phenols are reacted withcyanogen chloride, ClCN, and base to give the resins. In the cure step the cyanategroups trimerize to form triazine rings when heated in the range 180–250◦ C. Per-formance is generally intermediate between aromatic amine cured epoxides andtoughened bismaleimides. Glass transition temperature T g is about 250◦ C and theheat distortion temperature is about 250◦ C dry and 175◦ C wet. Electrical proper-ties are excellent due to very low residual chlorine content. Principal applicationsare printed wiring boards and structural composites (Fig. 3) (43). Benzoxazine Resins. Benzoxazine resins are prepared by the reaction ofphenol, formaldehyde, and an amine. In one particular example a benzoxazine isprepared from bisphenol A, formaldehyde, and aniline to give 2,2 -bis(3-phenyl-4-dihydro-1,3,2-benzoxazine) propane. When heated to about 200◦ C the methylenebond to oxygen breaks and reforms onto the available ortho positions of adjacentmoieties to give dibenzylamine structures. Resin formulations have been devel-oped and formulated, in some cases with epoxy and phenolic resins to give ternarysystems with T g as high as 170◦ C (Fig. 4) (43–46).CureA typical resin has an initial molecular weight of 150 to perhaps 1500. Forsystems of unsubstituted phenols, the ﬁnal cross-link density is 150–300 amu
336 PHENOLIC RESINS Vol. 7 Fig. 3. Curing via cyclotrimerization; R = bisphenol unit. From Ref. 43. Fig. 4. Polymerization reaction of benzoxazine resins.per cross-link. In other words, 25–75% of the ring-joining reactions occur duringthe cure phase. Resoles. The advancement and cure of resole resins follow reaction stepssimilar to those used for resin preparation; the pH is 9 or higher and reaction tem-perature should not exceed 180◦ C. Methylol groups condense with other methylolsto give dibenzyl ethers and react at the ortho and para positions on the phenol togive diphenylmethylenes. In addition, dibenzyl ethers eliminate formaldehyde togive diphenylmethanes. In some resole applications, such as foam and foundry binders, a rapid cure ofa liquid resin is obtained at room temperature (RT) with strong acid. The reactionsproceed in the same manner as those of novolak resin formation. Methylol groupsreact at ortho and para phenolic hydrogen to give diphenylmethane units (47). At pH 4–6, the cure is slower than it is at pH 8 and higher, and much slowerthan at pH 1–3. Reactions at pH 4–6 resemble those on the more alkaline side,
Vol. 7 PHENOLIC RESINS 337but with a substantial increase in side products. This is partly the result of thelow rates of the main reactions and partly the result of stable intermediates atthis pH range. Some resoles contain latent acid catalysts, which on heating generate mod-erately strong acids. Examples include aryl phosphites such as diphenyl hydrogenphosphite and ammonium sulfate (48,49). The use of latent acid catalysis broad-ens the range of applications of phenolic resins to include areas such as liquidcomposite molding and pultrusion. Also resoles, which can contain so-called freeformaldehyde, can be formulated with formaldehyde scavengers in form of aminessuch as melamine. Novolaks. Novolak resins are typically cured with 5–15% hexa as thecross-linking agent. The reaction mechanism and reactive intermediates havebeen studied by classical chemical techniques (3,4) and the results showed thatas much as 75% of nitrogen is chemically bound. More recent studies of resin cure(50–53) have made use of TGA, DTA, GC, IR, and NMR (16). They conﬁrm that thecure begins with the formation of benzoxazine (12), progresses through a benzylamine intermediate, and ﬁnally forms (hydroxy)diphenylmethanes (DPM). In the reaction of phenol and bisphenol F with hexa, NMR spectra show thetransient appearance of benzoxazine intermediates; after 2 h at 103◦ C, all the ben-zoxazine decomposed to the diphenylmethylene and benzylamine intermediates(16). The cure of novolaks with hexa has been studied with differential scanningcalorimetry (DSC) and torsional braid analysis (TBA) (54); both a high ortho no-volak and a conventional acid catalyzed system were included. The DSC showedan exothermic peak indicating a novolak–hexa reaction ≈20◦ C higher than thegelation peak observed in TBA. Activation energies were also calculated. The resin rich in 2,2 -methylene exhibited the lowest activation energy, geltemperature, and DSC exotherm. The high concentration of the slightly acidic2,2 -diphenylmethane end groups may account for the higher reactivity. Theseend groups should react with hexa to form benzoxazine intermediates ﬁrst, whichthen decompose to react with vacant positions throughout the novolak molecule. An isothermal method for studying the cure of phenolics employs dynamicmechanical analysis (DMA) (Table 7). The problems associated with programmed
338 PHENOLIC RESINS Vol. 7 Table 7. Isothermal DMA Results Rate, min − 1 Sample At 150◦ C At 185◦ C Activation energy, kJ/mola Hexa-catalyzed resole 0.22 1.00 71.1 Novolak 6% hexa 0.07 0.09 8.8 12% hexa 0.12 0.19 18.8 a To convert kJ to kcal, divide by 4.184.heating rates are avoided and mathematical treatment of the results is simpliﬁed.Although a more complex treatment is possible, a simple ﬁrst-order dependence ofmodulus with time and an Arrhenius-type temperature dependence are sufﬁcient.The rate studies of Table 7 indicate that doubling the amount of hexa doubles therate at which the modulus approaches its long-term value. The novolak – 12% hexacures substantially slower than the resole. In addition, they differ in temperaturedependence of cure rates; the resole has an activation energy approximately fourtimes greater than that of the novolak – 12% hexa (55). Decomposition of Cured Resoles and Novolaks. Above 250◦ C, curedphenolic resins begin to decompose. For example, dibenzyl ethers such as 9 dis-proportionate to aldehydes (salicylaldehyde) and cresols (o-cresol). The aldehydegroup is rapidly oxidized to the corresponding carboxylic acid. In an analogous re-action in hexa-cured novolaks, tribenzylamines decompose into cresols and azome-thines, which cause yellowing. Substantial decomposition of phenolic resins begins above 300◦ C. In the pres-ence of oxygen, the methylene bridging group is converted to a hydroperoxide,which, in turn, yields alcohols and ketones on decomposition. The ketone is especially susceptible to random chain scission. Decomposition con-tinues up to ≈600◦ C; the by-products are mostly water, CO, CO2 , and phenols. Theﬁrst stage of decomposition produces a porous structure having minimal shrink-age. The second stage begins near 600◦ C and is accompanied by shrinkage andsubstantial evolution of CO2 , H2 O, methane, and aromatics. The resulting pol-yaromatic chars represent ≈60% of the original resin when the atmosphere isinert, but this may be substantially less in the presence of air. The char ignites inair above 900◦ C.
Vol. 7 PHENOLIC RESINS 339 The controlled decomposition of phenolic resins, in an inert atmosphere, is amethod used to make carbon–carbon composites. In this case the resin is combinedwith other forms of carbon, such as carbon ﬁbers, coke, and synthetic graphite,and cured under heat and pressure. Further heating to about 900◦ C converts theresin to a glassy form of carbon that can serve as a binder for the other carbonforms. The carbon yield from the phenolic resins can be in the range of 60–70% ofthe initial weight (see under CARBON–CARBON COMPOSITES).Analysis and CharacterizationThe principal techniques for determining the microstructure of phenolic resinsinclude mass spectroscopy (MS), proton and 13 C NMR spectroscopy, as well asGC, LC, and GPC. The softening and curing processes of phenolic resins are effec-tively studied by using thermal and mechanical techniques, such as TGA, DSC,and DMA. Infrared (IR) and electron spectroscopy are also employed. Recentlymatrix-assisted laser desorption-ionization mass spectrometry (MALDI-MS) hasbeen used for the determination of molecular weight and end-group analysis (seeMASS SPECTROMETRY). MALDI-MS is a soft ionization technique that has been ap-plied to the determination of mass of large biomolecules and synthetics resins.The approach is useful for molecular weight determination and end-group analy-sis. Both novolaks and resoles have been studied and individual fragments withm/z up to about 2000 speciﬁcally identiﬁed. For resoles the technique is even ableto resolve the various hemiformal structures that can occur. (Ref. 9, p. 92; 56–58). Spectroscopy. Infrared spectroscopy (59) permits structural deﬁnition,eg, it resolves the 2,2 - from the 2,4 -methylene units in novolak resins. However,the broad bands and severely overlapping peaks present problems. For uncuredresins, NMR rather than IR spectroscopy has become the technique of choice formicrostructural information. However, Fourier transform infrared (FTIR) givesuseful information on curing phenolics (60). Nevertheless, IR spectroscopy con-tinues to be used as one of the detectors in the analysis of phenolics by GPC. (seeVIBRATIONAL SPECTROSCOPY) A great wealth of microstructural information is provided by Fourier trans-form 13 C NMR. Using the much greater chemical-shift range of this technique,detailed structural information is provided for both the aliphatic and the aro-matic carbons (Table 8). Current techniques provide highly reliable quantitativedata and relative peak areas (19,61–65) and make possible a quantitative mea-sure of the numbers of branch points and end groups. Branching can cause earlygelation in a novolak resin, and end groups usually have greater reactivity in thethermosetting reaction than do the backbone units. Another important advantageof 13 C NMR is the parametric predictability of the chemical-shift values. As a re-sult, unknown peaks can be assigned to a hypothetical structure with reasonablecertainty. At the same time, the process can be reversed and a computer can pro-vide detailed structural analysis. 13 C NMR has been applied to cured phenolicresins (63). (see NUCLEAR MAGNETIC RESONANCE). Chromatography. Gel-permeation chromatography (GPC) is an invalu-able technique for determining the molecular size distribution of polymers. Phe-nolic resins, which have molecular weight components ranging from 100 to rarely
340 PHENOLIC RESINS Vol. 7 Table 8. Chemical Shifts of Methylene Carbons in Liquid Resoles Structurea Chemical shift,b ppm Methylol C in 8 61.3 65.4 (b) ) 88.0 (c) Benzyl C in 9 68.9 Methylol C in 11 63.8 68.5 (d) 88.0 (e) 71.5 Methylene C in 5 31.5 Methylene C in 6 35.0 Methylene C in 7 40.4 a Designated carbon is shown in italic or described. b From tetramethylsilane in d6 -acetone solution.more than 5000, require special column arrangements to optimize resolution. Byusing proper instrument calibration, it is possible to obtain number-average (M n )and weight-average (M w ) molecular weight as well as quantitative informationon free monomer and certain other low molecular weight species (66–68) (seeCHROMATOGRAPHY, SEC). Many resole resins exist as phenolate salts in solution. Because these ionicspecies are sparingly soluble in carrier solvents such as tetrahydrofuran, carefulneutralization and ﬁltration are required. Although GPC is an excellent tech-nique for examining medium and high molecular weight fractions, GC and highperformance LC are more effective for analyzing low molecular weight species. Gas chromatography (GC) has been used extensively to analyze phenolicresins for unreacted phenol monomer as well as certain two- and three-ringconstituents in both novolak and resole resins (69). It is also used in moni-toring the production processes of the monomers, eg, when phenol is alkylatedwith isobutylene to produce butylphenol. Usually, the phenolic hydroxyl must bederivatized before analysis to provide a more volatile compound. The GC anal-ysis of complex systems, such as resoles, provides distinct resolution of over20 one- and two-ring compounds having various degrees of methylolation. Insome cases, hemiformals may be detected if they have been properly capped(61). The combined techniques of GC/MS are highly effective in identifying thecomposition of various GC peaks. The individual peaks enter a mass spectrometer
Vol. 7 PHENOLIC RESINS 341 Table 9. Resole Components by HPLC and GC Resina Components 2; 4; 2,4; 2,6; 2,4,6 2; 2,6; 2,2 ; 2,6,2 ; 2,6,2 , 6 2 ; 6; 4; 2 , 6 ; 6,2 ; 4,2 ; 4,6; 4,2 , 6 ; 4,6,2 ; 4,6,2 ,6 a Also, 5, 6, and 7, ie. 2,2 -, 2,4 -, and 4,4 -DPM.in which they are analyzed for parent ion and fragmentation patterns, and theindividual components of certain resoles are completely resolved. High performance liquid chromatography (HPLC) is extremely effective inseparating individual resin components up to a molecular weight of 1000 accord-ing to size and polarity. Dilute-solution conditions and low temperatures preservethe structure of unstable components. The resins are usually not derivatized. Gra-dient solvent elution gives excellent peak separation (69,70). In one study, resolescatalyzed by sodium and barium hydroxide were compared, and the componentswere separated up to and including methylolated four-ring compounds (61). Resolecomponents resolved by GC and HPLC techniques are shown in Table 9. Like GC,HPLC is most effective when combined with other analytical tools, such as massand UV spectroscopy. By using preparative-scale HPLC, individual peaks can beanalyzed by proton and 13 C NMR spectroscopy. Thermal Analysis. The main thermal analysis techniques applied to phe-nolic resins are TGA and DSC. In TGA, the sample weight is monitored microan-alytically with time and temperature in air or nitrogen. When applied to resinsand molding compounds, the scans indicate cure and decomposition temperaturesaccompanied by a measurable loss in weight. Resoles and novolaks lose from 5 to20% of their weight on curing at 100–200◦ C. Weight loss provides information onshrinkage, void formation, and density change of composites. Phenolic resins give a high char yield on combustion and TGA provides ameasure of the expected yield. Typical values are between 40 and 65% in nitrogen.Decomposition begins at 350◦ C and continues up to 600◦ C. Autoignition tempera-ture in air is above 900◦ C. Thermogravimetric analyses have played an importantpart in the development of carbon–carbon and carbon–graphite-ﬁber composites
342 PHENOLIC RESINS Vol. 7containing phenolic resins. These composites are used in aircraft brake liningsand carbon-pipe applications. In DSC and DTA, heat ﬂow and sample temper-ature are compared to a reference material. Glass-transition temperature T g isdetermined by DSC. The T g of liquid resoles is below RT, that of friable novolaksis in the range of 50–75◦ C, and that of lightly cross-linked phenolics is between150 and 225◦ C. Cure kinetics of thermosets are usually determined by DSC (71,72). How-ever, for phenolic resins, the information is limited to the early stages of the curebecause of the volatiles associated with the process. For pressurized DSC cells, theupper limit on temperature is ≈170◦ C. Differential scanning calorimetry is alsoused to measure the kinetics and reaction enthalpies of liquid resins in coatings,adhesives, laminations, and foam. Software packages that interpret DSC scans interms of the cure kinetics are supplied by instrument manufacturers. Dynamic Mechanical Analysis. In DMA, a vibrating or oscillating sam-ple is heated at a programmed rate or held isothermally at elevated temperature.The frequency and damping characteristics of the sample are monitored withtime. A change such as gelation or passage through the T g causes abrupt changesin the fundamental oscillation frequency of the sample and the damping abilityof the specimen. The oscillation frequency can be related to the storage modu-lus of the sample, whereas the damping contains information related to the lossmodulus. Softening and cure are examined with the help of a torsional pendulummodiﬁed with a braid (73), which supports thermosets such as phenolics andepoxies that change from a liquid to a solid on curing. Another method uses vi-brating arms coupled to a scrim-supported sample to measure storage and lossmoduli as a function of time and temperature. An isothermal analytical methodfor phenolic resins provides data regarding rate constants and activation ener-gies and allows prediction of cure characteristics under conditions of commercialuse (55). DSC and DMA scans of a novolac cure are shown in Figures 5a and 5b (74).The sample is a glassy solid initially and the DMA shows the distinctive T g at 65◦ Cfollowed by the appearance of a liquid state. From 110 to 125◦ C, the resin is a liquidand the chemical curing reactions begin, and it is followed by gelation at 140◦ C.Further reaction continues until 200◦ C, when a highly cross-linked, infusible solidis obtained. As the sample is cooled to RT, a slight increase in storage modulusis observed. The peak in the damping curve indicates the T g of the cross-linkedsystem at about 185◦ C. Dynamic mechanical analysis provides a useful technique to study the curekinetics and high temperature mechanical properties of phenolic resins. Thevolatile components of the resin do not affect the scan or limit the temperaturerange of the experiment. However, uncured samples must be supported by a braid,a scrim, or paper. This does not inﬂuence the kinetic results and can be correctedin the calculations of dynamic mechanical properties (qv). Recent DMA work onphenolic resins has been used to optimize the performance of structural adhesivesfor engineered wood products and determine the effect of moisture in wood producton cure behavior and bond strength (75–77). Control Tests. Numerous chemical and physical tests are used in themanufacture of phenolic resins to ensure correct properties of the ﬁnished resins,
Vol. 7 PHENOLIC RESINS 343 −400 −600 Heat flow Q, µW −800 3 1 −1000 −1200 2 −1400 0 50 100 150 200 250 Temperature, °C (a) 104 300 G′ (after curing) 250 Shear modulus G′, MPa G′ Loss modulus G′′ MPa 103 (original) 200 150 G′′ (original) 102 100 50 G′′ (after curing) 101 0 0 50 100 150 200 250 Temperature, °C (b)Fig. 5. DSC and DMA of novolac resin. (a) DSC Measurement of (1) original PF resin, (2)cured PF resin, and (3) novolac. (b) Torsion pendulum measurement of original and curedPF. To convert MPa to psi, multiply by 145. From Ref. 74.including the following: refractive index is used to estimate the dehydration duringmanufacture and is proportional to the solids content; viscosity is used to deter-mine molecular weight and solids content; nonvolatiles content is roughly propor-tional to polymer content; miscibility with water depends on the extent of reactionin resoles; speciﬁc gravity is measured for liquid resins and varnishes; meltingpoint of novolaks and solid resoles affects application performance; gel times de-termine the reactivity of the resins; resin ﬂow is a measure of melt viscosity andmolecular weight; particle size affects performance and efﬁciency; and ﬂash pointand autoignition temperature provide ﬂammability-characteristic measurements
344 PHENOLIC RESINS Vol. 7required by government agencies regulating safety and shipping. ASTM D4706-93 (1998) describes the standard test method for qualitative determination ofmethylol group in phenolic resins.Health, Safety, and Environmental FactorsThe factors contributing to the health and safety of phenolic resin manufactur-ing and use are those primarily related to phenol (qv) and formaldehyde (qv).Unreacted phenol in a resin can range from ∼5% for liquid resoles used in im-pregnation processes to well below 1% for novolaks intended for use as epoxyhardeners. Free formaldehyde can be <1% in liquid adhesives. Novolaks are usu-ally free of formaldehyde. The toxicity of the resins is signiﬁcantly lower than thatof the phenol and formaldehyde starting materials. No detrimental toxicologicaleffects have been reported for cured phenolic resins, which can be used in directcontact with food as in can coatings. Uncured resins are skin sensitizers and contact should be avoided, as well asbreathing the vapor, mist, or dust. Novolak-based pulverized products generallycontain hexamethylenetetramine, which may cause rashes and dermatitis. Phe-nolic molding compounds and pulverized phenolic adhesives must be controlled aspotentially explosive dusts. In addition, they contain irritating or toxic additives.ASTM test method D4639-86 (1996) describes the method for volative content inphenolic resins. Phenol. Phenol is highly irritating to the skin, eyes, and mucous mem-branes in humans after acute inhalation or dermal exposures. Phenol is consid-ered to be quite toxic to humans via oral exposure, with blood changes, liver andkidney damage, and cardiac toxicity reported. Chronic inhalation exposure to phe-nol in humans has been associated with gastrointestinal irritation, liver injury,and muscular effects. No data are available on the developmental or reproductiveeffects of phenol on humans. EPA has classiﬁed phenol as a Group D, not classi-ﬁable as to human carcinogenicity. The NIOSH threshold limit value (TLV) andOccupational Safety and Health Administration (OSHA) permissible exposurelimit for phenol is 19 mg/m3 (78). The health and environmental risks of phenoland alkylated phenols, such as cresols and butylphenols, have been reviewed (79). Formaldehyde. Acute and chronic inhalation exposure to formaldehydein humans can result in eye, nose, and throat irritation and respiratory symptoms.Reproductive effects have been reported in women workers exposed to formalde-hyde. Limited human studies have reported an association between formaldehydeexposure and lung and nasopharyngeal cancer. The EPA has classiﬁed formalde-hyde as a Group B1, probable human carcinogen of medium carcinogenic hazard.The OSHA has set its permissible exposure limit (PEL) at 4.5 mg/m3 and theAmerican Conference of Governmental and Industrial Hygienists have set theTLV at 1.5 mg/m3 (80). Wastewater. Phenol is a toxic pollutant to the waterways and has anacute toxicity (∼5 mg/L) to ﬁsh. Chlorination of water gives chlorophenols, whichimpart objectionable odor and taste at 0.01 mg/L. Biochemical degradation ismost frequently used to treat wastewater containing phenol. Primary activatedsludge, along with secondary biological treatment, reduces phenol content to below
Vol. 7 PHENOLIC RESINS 3450.1 mg/L (81). ASTM D1783-01 describes the standard test methods for phenoliccompounds in water. Flammability. Phenolics have inherently low ﬂammability and relativelylow smoke generation. For this reason they are widely used in mass transit, tunnelbuilding, and mining. Fiber-glass reinforced phenolic composites are capable ofattaining the 1990 U.S. Federal Aviation Administration (FAA) regulations fortotal heat release and peak heat release for aircraft interior facings (1,82). Theyare also used as “ﬁre restricting material” on cruise ships, high speed ferries,and commercial submarines. The self-ignition temperature is about 600◦ C andlimiting oxygen index (LOI) is in the range 40–49%. (83). Recycling. Thermosets are inherently more difﬁcult to recycle than ther-moplastics, and thermosetting phenolics are no exception. However, research inthis area has been reported, and molded parts have been pulverized and incor-porated at 10–15% in new molding powders. Both German and Japanese groupshad instituted this type of practice in 1992 (84,85) (see RECYCLING). A number of alternatives will have to be developed in order to effectivelyutilize cured phenolic material (86). One approach is the “thermoset recyclingpyramid,” a preferred order of execution that includes (1) Tier 1: Reintroduction of the used material into the original material at relatively low levels (∼10%) in the raw material mix (this approach is used widely to recycle SMC and BMC thermoset polyesters) (2) Tier 2: Reuse of the material in a lower performance thermoset product at relatively high levels (40–50%) (3) Tier 3: Reuse of the product in alternative materials such as asphalt, rooﬁng materials, concrete, and other construction products (4) Tier 4: Pyrolysis of the material to generate raw material feed stocks and incineration for energy recovery. Phenolic molding compounds can yield a caloric value of 14,000–23,000 kJ/kg, depending on the type of ﬁller. Plenco and other companies have been working with the SPI’s Phenolic Di-vision to produce a “Recycling Blueprint” shown in Figure 6 below (87). Biomass and Biochemical Processes. Phenolic resins have been pro-duced from biomass and using biochemical processes in various ways. In Japanbiomass from wood waste or waste from the food industry is treated with phenolsand strong acid catalysis and heat to produce phenolic resins (88). Research atthe National Renewable Energy Laboratory has shown that ablative fast pyroly-sis can be used to convert a wide variety of biomass feedstocks into a liquid oil.The phenolic rich component can be extracted from this oil and used as a low costreplacement for synthetic phenol in phenolic resins (89). In another approach, soy-bean peroxidase enzymes have been used to prepare resins from phenolic moietieswithout the use of formaldehyde (90). Economic Aspects. In 2000, worldwide consumption of phenolic resinsexceeded 4 × 106 t; slightly less than half of the total volume was produced inthe United States (91). The largest-volume application is in plywood adhesives,an area that accounts for ≈49% of U.S. consumption (Table 10). All wood bondingapplications account for about two-third of phenolic resin use. During the early
346 PHENOLIC RESINS Vol. 7 Table 10. Long-Term Use of Phenolic Resins,a 103 t End use market 1983 1993 2001 Bonding 295 454 645 Laminating 67 78 111 Plywood 580 687 976 Other 173 173 248 Total 1115 1392 1980 a Ref. 91. Source Reduction Identification/Collection/End-Use Determination Course Grind Sort & Clean Primary Recycle Secondary Recycle Tertiary Recycle Fine Grind Recycle into Other Uses, Thermal Treatment i.e. Asphalt Recycle into Same Product Recycle via Pyrolysis Recycle via Energy Recovery Recycle into Lower Grade Product Fig. 6. SPI Blueprint for the reclamation of molded phenolics.1980s, the volume of this application more than doubled as mills converted fromurea–formaldehyde (UF) to phenol–formaldehyde adhesives because of the releaseof formaldehyde from UF products. As a mature industry, U.S. production and application of phenolic resins haveparalleled the growth in the GNP and the housing industry. The consumption ofphenolic resins for coatings and molding powders has continued its decrease. Thedriving force behind coatings has been the need to reduce the volatile organicscontent (VOC) and the growth in alternative coatings such as waterborne, pow-der, and radiation-cured coatings. In the area of molding powders, numerous newengineering thermoplastics and alloys having superior properties have been in-troduced since the 1970s; however, phenolic molding powders continue to be usedextensively in electrical, electronic, and machinery and underhood parts applica-tions. U.S. phenolic resin manufacturers include Ashland, Borden Chemical, CytecFiberite, Durez, FiberCote Industries, H.B. Fuller, P.D. George, Georgia-Paciﬁc,
Vol. 7 PHENOLIC RESINS 347International Paper, Lockport Thermosets, Maruzen America, Plastics Engineer-ing, Resinoid, Sumitomo America, TriQuest, and Vantico (92). Prices of phenolic resins vary substantially depending on the application.In 2001, the price of general-purpose and semisolids was $1.50–1.80/kg, whereasepoxy-hardener grades can exceed $2.20/kg. Because raw materials of phenolicresins are derived from crude oil and natural gas, the prices of phenolic resinsdepend on the prices of these resources.Applications Coatings. For coatings applications, phenolic resins are grouped into fourclasses, depending on heat reactivity and the type of phenol. Substituted phenolsare more compatible with oil and hydrocarbons, whereas heat-reactive resins re-quire polar solvents. Depending on its nature, the resin can be used alone or asa modifying resin that acts as an adhesion promoter, a chemical cross-linker, or ahardening agent. In these cases the primary resin may be an alkyd, polyester, orepoxy (93). Unsubstituted heat-reactive resins are designed for baked-on coatings andare usually not oil-soluble. They require strong solvents and although most are notwater-miscible, their low molecular weight, high formaldehyde content promoteswater miscibility. These resins are available as solids, viscous liquids, and solu-tions. Resins prepared with an alkaline catalyst and a slight excess of formalde-hyde over phenol are heat-reactive, but not as much as resole resins designed forﬁber bonding and paper impregnation. Recommended cure conditions are 30 minand 150◦ C. Heat-reactive resins are more compatible than oil-soluble resins with otherpolar-coating resins, such as amino, epoxy, and poly(vinyl butyral). They are usedin interior-can and drum linings, metal primers, and pipe coatings. The coatingshave excellent resistance to solvents, acids, and salts. They can be used over a widerange of temperatures, up to 370◦ C for short periods of dry heat, and continuouslyat 150◦ C. Strong alkalies should be avoided. The maximum recommended ﬁlm thickness is 25 µm. At greater thicknesses,volatiles from the curing reaction, mainly water and some formaldehyde and phe-nol, can cause defects. These coatings have excellent electrical insulation proper-ties, ie, up to 20 V/µm, because of low moisture absorption and low conductance.The coatings are hard with low ﬂexibility, depending on curing conditions and ﬁlmthickness. Phenolic baking coatings can be used for metal, ceramic, and plastic sur-faces. Applications include equipment for heating and air conditioning, chemicalprocessing, petroleum reﬁning, and water treatment. Some types are used in oil-well pipes and marine environments (94). Certain coatings can be used in foodand beverage processing, subject to regulations. The largest use of novolak resins in coatings is as a hardener for epoxy resins.The epoxy is frequently based on bisphenol A or epoxidized novolaks. Basic cata-lysts such as benzyldimethylamine are required for moderate baking conditions,such as 2 h at 180◦ C. The phenolic/epoxy ratio is adjusted to be stoichiometri-cally equivalent in order to give a highly cross-linked coating that has moderate
348 PHENOLIC RESINS Vol. 7ﬂexibility and excellent resistance to chemicals, heat, and moisture. Powder coat-ing of pipes continues to be a growing application, especially when corrosion resis-tance is required. In solution form, the epoxy–phenolic systems are used as metalprimers and in pipe coating. Substituted heat-reactive resins are most widely used in contact-adhesiveapplications and, to a lesser extent, in coatings (95,96); p-butylphenol, cresol, andnonylphenol are most frequently used. The alkyl group increases compatibilitywith oleoresinous varnishes and alkyds. In combination with these resins, pheno-lics reduce water sensitivity. Common applications include baked-on and electricalinsulation varnishes, and as modiﬁers for baking alkyds, rosin, and ester gum sys-tems. Substituted heat-reactive resins are not used for air-dry coatings becauseof their soft, tacky nature in the uncured state; substituted nonheat-reactive phe-nolics are the modifying resin of choice in this case. Substituted nonheat-reactive resins do not form a ﬁlm and are not reactiveby themselves, but are excellent modiﬁer resins for oleoresinous varnishes andalkyds. Their high T g and molecular weight provide initial hardness and reducetack; oxygen-initiated cross-linking reactions take place with the unsaturatedoils. Early phenolic resin drying-oil varnishes were cooked in order to incorporatethe phenolic resin into the formula. These resins have been replaced by cold-cutresins that reduce atmospheric emission by permitting direct incorporation ofthe phenolic after the oleoresinous varnish has been prepared. High solids sys-tems enable coatings to meet the VOC standards required by regulatory agencies.Newer phenolic varnishes, developed in the 1980s, may contain as high as 80%nonvolatile solids (97). Oleoresinous phenolic varnishes are excellent coatings that dry in 2–4 hand show exterior durability, corrosion resistance (especially when aluminum-modiﬁed), compatibility, solubility, and good package stability. Recoatability andintercoat adhesion are also excellent. The ﬁlms are sensitive, however, to strongsolvents and concentrated acids and alkalies. Unlike systems containing cross-linking phenolics, ﬁlms containing these resins remain ﬂexible. Phenolics that are not heat-reactive may be incorporated into both air-driedand baked oleoresinous coatings. Applications vary widely and include clear andpigmented exterior varnishes, aluminum-maintenance paints, zinc-rich primers,can coatings, insulation varnishes, and concrete paints. As modiﬁers in a greatvariety of applications, they enhance the performance of oleoresinous and alkydcoatings. Dispersions. In phenolic resin dispersions, the continuous phase is wateror a nonpolar hydrocarbon solvent. The resin exists as droplets that have particlesizes of 1–20 µm and are dispersed in the continuous phase. Aqueous dispersionsare prepared either in situ during the preparation of the resin itself or by highshear mixing (26,37). Aqueous dispersions are alternatives to solutions of liquid and solid resins.They are usually offered in 50% solids and may contain thickeners and cosolventsas stabilizers and to promote coalescence. Both heat-reactive (resole) and nonheat-reactive (novolak) systems exist that contain unsubstituted or substituted phenolsor mixtures. A related technology produces large, stable particles that can beisolated as discrete particles (52). In aqueous dispersion, the resin structure is
Vol. 7 PHENOLIC RESINS 349designed to produce a hydrophobic polymer, which is stabilized in water by aninterfacial agent. Aqueous dispersions are used in ﬁber bonding, paper coating, friction andabrasive applications, and laminates and wood bonding. Phenolic dispersions im-prove the strength of latex-contact adhesive applications. Epoxy-modiﬁed phenolicdispersions are prepared by dispersion of the phenolic epoxy resin. The systemsare used for baked primer applications and bonding requirements. Minimum bak-ing conditions are 20 min at 150◦ C (26). Adhesives. Contact adhesives are blends of rubber, phenolic resin, andadditives supplied in solvent or aqueous dispersion form; they are typically appliedto both surfaces to be joined (98). Evaporation of the solvent leaves an adhesive ﬁlmthat forms a strong, peel-resistant bond. Contact adhesives are used widely in thefurniture and construction industries and also in the automotive and footwearindustries. The phenolic resins promote adhesion and act as tackiﬁers, usuallyat a concentration of 20–40%. In solvent-based contact adhesives, neoprene ispreferred, whereas nitrile is used in specialty applications. The type and grade ofphenolic resin selected control tack time, bond strength, and durability. Neoprene–phenolic contact adhesives, known for their high green strengthand peel values, contain a resole-type resin prepared from 4-t-butylphenol. Thealkyl group increases compatibility and reduces cross-linking. This resin reactsor complexes with the metal oxide, eg, MgO, contained in the formulation, andincreases the cohesive strength of the adhesive. In fact, the reactivity with MgOis frequently measured to determine the effectiveness of heat-reactive phenolicsin the formulation. Phenolic resins substantially increase open time and peel strength of theformulation (98). For example, higher methylol and methylene ether contents ofthe resin improves peel strength and elevated temperature resistance. Adhesiveproperties are also inﬂuenced by the molecular weight distribution of the phenolic;low molecular weight reduces adhesion (99). Waterborne contact adhesives contain an elastomer in latex form, usually anacrylic or neoprene-based latex, and a heat-reactive, cross-linkable phenolic resinin the form of an aqueous dispersion. The phenolic resin improves metal adhesion,green strength, and peel strength at elevated temperature. A typical formulationcontains three parts latex and one part phenolic dispersion (dry weight bases).Although metal oxides may be added, reaction of the oxide with the phenolic resindoes not occur readily.
350 PHENOLIC RESINS Vol. 7 Bonding properties of water-based contact adhesives are similar to thoseof solvent-based systems, but are free of ﬂammability hazards. However, dryingtimes are longer and the bond is sensitive to moisture. Carbonless Copy Paper. In carbonless copy paper, also referred to aspressure-sensitive record sheet, an acid-sensitive dye precursor, such as crystalviolet lactone or N-benzoylleucomethylene blue, is microencapsulated with a highboiling solvent or oil within a cross-linked gelatin (94,100,101) or in syntheticmononuclear microcapsules. Microcapsules that have a starch binder are coatedonto the back of the top sheet. This is referred to as a coated-back (CB) sheet. Thesheet intended to receive the image is treated on the front (coated-front (CF)) withan acid. When the top sheet is mechanically impacted, the dye capsules ruptureand the dye solution is transferred to the receiving sheet where the acid developeractivates the dye. The original acid–clay developers have been largely replaced by phenoliccompounds, such as para-substituted phenolic novolaks. The alkyl group on thephenolic ring is typically butyl, octyl, nonyl, or phenyl. The acidity is higher thanthat of a typical unsubstituted novolak because of the high concentration of 2,2 -methylene bridges. Color intensity and permanence are improved by metal carboxylate salts,especially zinc salts (100), which catalyze the dye development and stabilize thedye in its colored form. The substituted novolak resin, along with extender andbinder, can be applied to the receiving sheet as a solution or aqueous dispersion.Aqueous dispersions are probably the most widely used; they are manufacturedby the resin supplier or the user from the base resin. A typical coating composition for the CF component is shown in Table 11. Itis dried in a high velocity air oven at 93◦ C. Molding Compounds. Molding compounds were among the earliest ap-plications for solid phenolic resins. Molding neat phenolic resin was almost im-possible and the strength, especially on impact, was poor without reinforcement.Combining the resin, usually a novolak, with hexa, wood-ﬂour, or asbestos rein-forcement, as well as pigments and additives, gave a moldable thermoset. Themolded articles exhibit high temperature, ﬂame, and chemical resistance, reten-tion of modulus at elevated temperature, and hardness. Systems that have goodelectrical properties can be formulated at low cost. Resins can be compoundedwith a choice of ﬁllers for a variety of applications. ASTM D4617-96 is the speciﬁcation that covers phenolic molding compounds.The general-purpose compounds, having good strength and electrical properties, Table 11. CF Coating Slurry Formulation Constituent Parts Kaolin clay 64 CaCO3 3 Colloidal silica 5.4 Hydroxyethyl starch 3 Styrene–butadiene latex 12 Novolak resin dispersion 12
Vol. 7 PHENOLIC RESINS 351Table 12. Applications for Molded Phenolic PartsaMarket Key features ExamplesAppliances Heat, moisture and Coffee pot handle and base; chemical resistance; steam iron parts thermal and electrical insulationAutomotive and Heat, moisture, and Disc brake caliper pistons, transportation hydrocarbon resistance; transmission parts; water dimensional stability pump parts, torque converters; oil pump coversElectrical Heat and wear resistance; Circuit breakers; motor thermal and electrical control parts; commutators insulation and alternatorsAerospace Heat and chemical Interior partitions; ablative resistance; rigidity surfacesPackaging Dimensional stability; Closures chemical resistancea Ref. 102.are used in electrical appliances, automotive ignitions, and handles. Impact-resistant grades contain longer glass and textile ﬁbers and rubber modiﬁers. Ap-plications include pump housing and switches. Heat resistance is improved byincorporating mineral and glass ﬁllers. Electrical-grade compounds contain micaand ﬁber glass ﬁllers, and are used in specialty switches and cases. Graphiteﬁller reduces the coefﬁcient of thermal expansion. Although phenolic moldingcompounds compete with a wide variety of thermoset and thermoplastic com-pounds, they continue to be the preferred material in numerous applications,such as reinforced phenolic pistons in automotive disk brakes and transmis-sion torque converters. Table 12 lists several applications for molded phenolicparts. Phenolic molding materials are prepared by ﬁrst blending the pulverized rawmaterials. In a compounding operation, the blend is passed through heated rollsto form a sheet as the resin melts. The compounded mixture remains on heatedrolls until the desired ﬂow and viscosity are reached. At this point, it is dischargedas a thin sheet and allowed to cool. The product is then granulated and packaged.Alternatively, a Banbury-type mixer can be used for the initial mixing; the mix isthen fed to a roll mill for ﬁnishing and sheeting. Compounding extruders are alsoused and through a continuous process provide a pelletized product. Phenolic resins used in molding materials are predominantly novolaks withhexa as the curing agent. Oxalic acid catalyzed novolaks and high ortho resinsare used. Resole resins may be used in place of hexa as the curing agent in certainelectrical applications in which the NH3 generated from the hexa can adversely af-fect metals such as copper and silver. Typically, the compound contains 40–50 wt%resin binder, 40–45% ﬁller, and 5–10% pigment and additive. Fillers and reinforce-ments include wood ﬂour, nutshell ﬂour, cellulose ﬁber, mica (qv), wollastonite,mineral wool, mineral ﬂour, glass ﬁber, organic ﬁber, carbon ﬁber, clay, andtalc. Additives and pigments are magnesium oxide, graphite, molybdenum
352 PHENOLIC RESINS Vol. 7sulﬁde, stearates, calcium carbonate, carbon black, nigrosine, lime, ﬂuoropoly-mers, and salicylic acid. Molding materials are fabricated into articles by compression, transfer, andinjection molding processes. For compression molding, the powder is poured intothe mold cavity or a preform heated prior to molding. Temperature ranges from140 to 190◦ C and pressures from 13.8 to 55.5 MPa (2000–8000 psi). Because thematerial is more ﬂuid in the mold, transfer molding is suitable for molding aroundinserts or for intricate shapes. In injection molding, cross-linking in the barrel andsprues must be avoided. Abrasives. Abrasive materials are either bonded or coated. Bonded phe-nolic abrasives have superior strength and shock resistance compared to sinteredceramic compositions. The higher stability permits higher rotational speeds forresin-binder wheels; however, temperatures are lower than with ceramic wheels. Synthetic aluminum oxide and silicon carbide are the principal inorganicabrasive materials. They are used in grit sizes from 44 or ﬁner to 1680 µm (12–325 mesh). The coarser grit sizes are used for rough work when wheels are as largeas 60 cm in diameter and 7.5-cm thick. These wheels are mounted in swinging-frame grinders and used to remove surface imperfections from stainless steelbillets. Finer grit (250 µm (60 mesh)) may be used in 45-cm-dia cutoff wheelsmounted in automatic grinders. These wheels can slice through a solid 2.5-cmsteel bar in 4 s, leaving a clean, shiny cut surface. In the usual method of manufacture, the grit is ﬁrst wetted with a low vis-cosity liquid resole phenolic resin or furfural, using 1–3 wt% of the grit. A drymixture of phenolic resin and ﬁllers is added and the combination of wet grit andpowder is tumbled until each grit particle is coated. The mix is temporarily dryand free-ﬂowing. The powdered phenolic resin varies from 6 to 10% of the weightof the grit. The quantity and type of ﬁller (alumina, cryolite, iron oxide, silicate)depend on the intended use of the wheel, whose grinding characteristics are af-fected by the ﬁller. The free-ﬂowing grit resin mix is placed into the mold andpressed at RT for 1–2 min at 13.8–34.5 MPa (2000–5000 psi). The dense form isremoved and cured for 12–24 h; temperatures are increased gradually to 185◦ Cfor 8–12 h. Pressing temperatures may be increased for high density structures. Heat resistance is an important characteristic of the bond. The strengthof typical abrasive structures is tested at RT and at 300◦ C. Flexural strengthsare between 24.1 and 34.4 MPa (3500–5000 psi). An unmodiﬁed phenolic resinbond loses about one-third of its RT strength at 298◦ C. Novolak phenolic resinsare used almost exclusively because these offer heat resistance and because themoisture given off during the cure of resole resins results in undesirable porosity.Some novolaks modiﬁed with epoxy or poly(vinyl butyral) resin are used for softergrinding action. Coated abrasives, such as sheets, disks, and drums, are used for polishingand ﬁnishing. Here, too, the abrasives, such as aluminum oxide and silicon carbide,have replaced the ﬂint and garnet of common sandpaper. These industrial coatedabrasives are manufactured from cloth or tough paper base. First, a coat of mediumviscosity liquid resole resin is laid down on a continuous web of the backing. Theweb passes wet-side-down over a pan of grit, which adheres to it electrostaticallyand remains embedded in the resin layer. Altering the strength of the appliedelectrostatic ﬁeld and the speed of the web can control the amount of grit deposited,
Vol. 7 PHENOLIC RESINS 353which varies from an open to a closed dense mass of abrasive. The uncured coatedsheet is partially dried in a low temperature oven at 60◦ C, and a second, thinnercoating of lower viscosity liquid resole resin is applied as a top to anchor thegrit thoroughly. The coated web is taken off in rolls to be cured at 107–120◦ C for3–4 h. The resins should dry quickly and cure well at low temperatures. They usu-ally are made at a high pH with high ratios of formaldehyde to phenol and heldto fairly low molecular weight. Typical viscosities are 15,000 mPa·s (=cP) at 75%solids content for a ﬁrst coat and 1000 mPa·s (=cP) at 50% solids for the top resin.For dense backing materials, such as ﬁber disks, a typical resin has a viscosity of50,000 mPa·s (=cP) at 80% solids and is cured at 148◦ C. New opportunities arearising for coated abrasive belts in high pressure grinding. High strength backinghas been developed and zirconia media are available for grinding. Friction Materials. Phenolic friction materials are made from moldingcompounds developed to meet the extraordinary demands required by frictionelements in the transportation industries. Friction materials are used for brakelinings, clutch facings, and transmission bands. A moderately high coefﬁcient offriction, which is temperature-independent, is needed. In addition, the materialmust be high in strength, low in wear and abrasion, and resistant to moisture andhydraulic ﬂuids. In the 1980s, signiﬁcant changes occurred in automotive brake elements.Reformation of friction elements eliminated asbestos and increased employmentof disk brakes. These developments required binder resins that have higher tem-perature performance without affecting the coefﬁcient of friction and wear. Alter-natives to asbestos include mineral, carbon, aramid, and metal ﬁbers, especiallyiron. Semimetallic linings contain as much as 70% iron ﬁbers. Other inorganicﬁllers include barites, alumina, lime, magnesia, and clay. Graphite and molybde-num disulﬁde are used to reduce scoring. The resins can be a novolak–hexa or a resole–novolak blend. In some applica-tions liquid resoles are used. Addition of alkylated phenol, oil, or cashew nutshellliquid (CNSL) reduces hardness and increases abrasion resistance. Modiﬁcationby rubber improves the coefﬁcient of friction and reduces brake fading. Many friction material formulations contain 5–15 wt% of friction particles,the granulated cross-linked products of the reaction of CNSL, a phenol substi-tuted at the meta position with a C15 , unsaturated side chain, and formaldehyde.Friction particles range in size from 50 to 500 µm. They reduce frictional wearand increase pedal softness (103). Manufacture of friction elements includes the impregnation of fabrics andsubsequent lamination, the wet-dough process, and the dry-mix process. Ele-ments from the last two are prepared by compression-molding the formulationfor up to an hour at 150–175◦ C. Thick brake elements require a carefully con-trolled heating-and-cooling cycle to minimize stresses created by expansion andcontraction. Foundry Resins. In the foundry industry, phenolic resins are used as thebinder for sand in the manufacture of shell molds and cores. The two mating halvesare joined by clamps or a bonding agent to form a shell mold into which the moltenmetal is poured for castings. The shell is formed by depositing a resin–sand mixon a hot metal pattern plate. After a certain period the pattern is inverted and
354 PHENOLIC RESINS Vol. 7the excess resin–sand is removed. The sand particles are bonded by an oven cure,and the shell is ejected from the pattern plate. Iron is the preferred metal for casting; steel and nonferrous metals are usedin smaller amounts. Most castings are made in green sand molds, ie, uncuredmolds of sand, clay, and water. However, the use of shell moldings is growing,because such moldings permit reproducibility of castings with close dimensionalaccuracy. In addition, the simplicity of equipment procedures reduces costs. The shell-molding process, introduced in the United States in 1948, is animportant market for phenolic resins. In the original process, dry sand andpowdered resin (6–8%) are blended. However, because of the high binder con-tent and the difﬁculty in obtaining a uniform mix, precoating methods weredeveloped. Both cold- and warm-coating processes employ solutions of phenolic resins.The principal process used for foundry resins is the hot-coating process. It is thefastest, least expensive, and safest process, and it requires no volatile removal.The sand is heated to 135–170◦ C in a muller, and solid novolak resin in ﬂakeform is added, which melts quickly and coats the sand. A lubricant may be addedat this point. After 1 min of mulling, the batch is cooled by adding water, whichevaporates rapidly. Hexa, which is not supplied with the resin, is usually added either with thewater as a solution or just before or immediately after the water addition. Byquenching the mix with water, the resin-coated sand is cooled to a point wherethere is no signiﬁcant reaction with the curing agent. Any reaction between theresin and the hexa in the muller affects the bonding properties of the coated sand.As the batch cools and begins to break up, more lubricant may be added, whichremains on the outside of the coated grains where it is most effective. The total cycle time for most production batches is 2.5–3.5 min, considerablyshorter than the cold- or warm-coating processes. Although a few available unitshave large capacity per batch, high production rates are possible because of theshort cycle. While one batch is being mulled, sand for the next batch can be heated.The typical ﬂake phenolic is an intermediate melting-point novolak containing 4%lubricant. Laminates. Laminate manufacture involves the impregnation of a webwith a liquid phenolic resin in a dip-coating operation. Solvent type, resin con-centration, and viscosity determine the degree of ﬁber penetration. The treatedweb is dried in an oven and the resin cures, sometimes to the B-stage (semicured).Final resin content is between 30 and 70%. The dry sheet is cut and stacked, readyfor lamination. In the curing step, multilayers of laminate are stacked or laid upin a press and cured at 150–175◦ C for several hours. The resins are generallylow molecular weight resoles, which have been neutralized with the salt removed.Common carrier solvents for the varnish include acetone, alcohol, and toluene.Alkylated phenols such as cresols improve ﬂexibility and moisture resistance inthe fused products. Industrial laminates are composed of two or more webs in sheet form thathave been impregnated with a thermosetting resin and molded under heat andpressure. The web is usually made of cellulose paper, cotton fabric, glass cloth,glass mat, asbestos paper, wood veneer, and similar materials. Laminates aremanufactured in sheets, rods, tubes, and special shapes, which can be machined by